DOI: 10.15632/jtam-pl.56.1.3

**HYGROTHERMOELASTIC BUCKLING RESPONSE OF COMPOSITE**
**LAMINATES BY USING MODIFIED SHEAR DEFORMATION THEORY**

Masoud Kazemi

*Environmental Sciences Research Center, Islamshahr Branch, Islamic Azad University, Islamshahr, Iran*
*e-mail: masoud kazemi@hotmail.com; kazemii@iiau.ac.ir*

In this study, a ﬁnite element based formulation is developed for analyzing the buckling and post-buckling of composite laminates subjected to mechanical and hygrothermal loads using Modiﬁed Hyperbolic Shear Deformation Theory (MHSDT). The changes in the critical buckling load are presented for diﬀerent lamination schemes, thicknesses, material properties and plate aspect ratios. In addition, post buckling analysis is performed for a composite plate subjected to uniform in-plane thermal and moisture induced loadings by using MHSDT. Matlab software has been used for programming the analysis. The results obtained by Matlab codes are in a satisfactory consistence compared to the references. Thus, the developed MHSDT has been validated for buckling and post buckling analysis of laminated plates in hygrothermal environment.

*Keywords:* angle-ply laminate, buckling, composite plate, ﬁnite element method, shear
de-formation theory

**1.** **Introduction**

Compared to conventional metal structures, ﬁbrous composite materials continue to experience increased application in aerospace, marine, automobile and other mechanical and civil structures due to their superior strength and stiﬀness to weight ratios; however, due to material anisotropy, analyzing and designing these materials are more complicated than metallic materials.

In order to prevent buckling and post-buckling eﬀects in laminated plates, using an extra--strength is of great practical importance in the structural design of laminated plates.

Buckling is known as one of the most critical failure modes, often pre-generated or produced
during service life. A signiﬁcant reduction in weight of laminated plates can be achieved
conside-ring the post buckling behavior, which is an important factor in aerospace structures. The elastic
buckling and post-buckling of ﬁber reinforced composite plates are investigated in several
*text-books (Agarwal et al., 2006; Reddy, 2004; Turvey and Marshall, 2012). Composite laminates are*
also susceptible to delamination buckling and exterior damage at stress free edges, which occurs
when the properties mismatch at the ply interface. It can also be produced by external forces,
elevated temperature and absorbed moisture. Stresses within laminates are redistributed to
re-duce the load carrying capacity, when delamination occurs. Composite laminates are subjected
to changing environmental conditions like temperature and moisture. The eﬀect of temperature
and moisture is known as thermal and hygroscopic eﬀect, respectively. The combined eﬀect of
these two parameters is called the hygrothermal eﬀect. A hygrothermal environment reduces
both strength and elastic properties, especially in the case of ﬁbrous polymeric composites.
Fur-thermore, associated hygrothermal expansion, either alone or in combination with mechanically
produced deformation, can result in buckling, large deﬂections, and high stress levels.
Conse-quently, examining the hygrothermal eﬀects is essential in analyzing and designing laminated
systems (Tauchert and Huang, 2012). Due to the fact that most applications are limited to
purely thermal loadings, the majority of published researches lie in this ﬁeld.

According to the similarities between mathematical formulations of the governing
ther-mal and hygroscopic loadings, the given thermoelastic solutions could be generalized to
elasto--hygrothermal cases. Similarly, it is not diﬃcult to simplify the hygrothermal formulations and
solution methods to include the isothermal eﬀects. For predicting the real behavior of a structure,
it is important to choose an adequate theory which is used in the expansion of diﬀerent variables
*(Mantari et al., 2012). In the 3D elasticity theory, heterogeneous laminated plates are modeled*
as 3D solid elements, so predicting transverse shear stresses can be signiﬁcantly improved,
ho-wever, by using this theory would lead to a complex procedure and multiplied computational
cost.

In the literature, diﬀerent models have been suggested for studying the composite laminated
structures, including layerwise, quasi-layerwise and equivalent single layer models. Three
prin-cipal equivalent theories have been proposed to reduce the 3D models to 2D ones; which are
known as the Classical Laminated Plate Theory (CLPT), First-order Shear Deformation Theory
*(FSDT) and Higher-order Shear Deformation Plate Theory (HSDT) (Kharazi et al., 2014).*

In the CLPT, which relies on the Love-Kirchhoﬀ assumptions, the transverse shear defor-mation is neglected and is only applicable for thin laminated plates, so, in order to consider the shear eﬀect, the FSDT based on Reissner-Mindlin theory has been developed. The FSDT is simple to perform and can be applied for both thick and thin laminates; however, the accuracy of solutions strongly relies on the shear correction factors. In addition, the FSDT would not give satisfactory results in predicting the accurate and smooth variations of stresses, speciﬁcally for laminated plates with clamped or free edges, sharp corners and highly skewed geometry where high stress gradients occur. To overcome the limitation of the FSDT, a simple higher order the-ory was presented by Reddy (2004) for laminated plates, various types of HSDT, which include higher order terms in Taylor’s expansion.

Many studies in the literature investigated the buckling and post-buckling in composite
la-minated thin plates subjected to mechanical or thermal loadings or both based on the classical
*plate theory, see for example (Kazemi and Verchery, 2016; Peković et al., 2015; Ahmadi and*
Pourshahsavari, 2016; Muc and Chwał, 2016). In some other studies (Girish and
*Ramachan-dra, 2005; Mechab et al., 2012; Dafedar and Desai, 2002), the application of shear deformation*
plate theories was developed for buckling and post-buckling analysis of laminated plates under
combined mechanical and thermal loading. It should be noted that in all these investigations,
the material properties are considered to be independent of temperature. Although
compre-hensive literature has been published in the ﬁeld of pure mechanical or pure thermal loadings,
few investigations have been devoted to the elastic buckling and post-buckling caused by
co-upled thermal and mechanical loads, which is encountered in real cases and operational life of
composite structures.

A reﬁned two-dimensional model was proposed by Brischetto (2013) for static hygrothermal
analysis of laminated composites and sandwich shells neglecting the transverse shear
deforma-tion eﬀects. Sreehari and Maiti (2015) introduced a ﬁnite element soludeforma-tion for handling buckling
and post buckling analysis of laminated plates under mechanical and hygrothermal loads using
a reﬁned HSDT; however, the accuracy of the method was veriﬁed only for cross-ply laminates.
*Natarajan et al. (2014) considered the eﬀect of moisture condensation and thermal variation on*
the vibration and buckling of laminates with cutouts within the formulation of the extended
*ﬁnite element method. Pandey et al. (2009) examined the inﬂuence of moisture concentration,*
temperature variation, plate parameters and ﬁber-volume fraction on the buckling and post
buc-kling of the laminated plates based on HSDT and von Karman’s nonlinear kinematics; however,
the distribution of temperature and moisture on the surface was assumed to be uniform.

The aim of present work is to analyze the buckling and post buckling behavior of composite laminated plates in hygrothermal environment using the Finite Element Method (FEM) based on a new higher order formulation, in which the displacement of the middle surface is developed

as a trigonometric and exponential function of thickness, and the transverse displacement is assumed to be constant through the thickness. An appropriate distribution of the transverse shear strain is assumed across the plate thickness and, also, the stress-free boundary conditions are considered on the boundary surface, therefore, a shear modiﬁcation factor is not needed.

**2.** **Trigonometric shear displacement model (TSDM)**

*A laminated plate consisting of N orthotropic plies is considered. Length, width and thickness*
*of the rectangular plate are a, b, and h, respectively. An 8-noded serendipity quadrilateral*
*element, which is C*0-continuous isoperimetric bi-quadratic, has been used for discretization of
the laminated plate. In this work, the following new displacement model is proposed to satisfy
the boundary conditions at the top and bottom of the laminated plate

*u(x, y, z) = u*0*(x, y) − z*
*∂w*
*∂x* +
h
sin*πz*
*h* exp
*m cosπz*
*h*
+ *π*
*hmz*
i
*θx(x, y)*
*v(x, y, z) = v*0*(x, y) − z∂w*
*∂y* +
h
sin*πz*
*h* exp
*m cosπz*
*h*
+*π*
*hmz*
i
*θy(x, y)*
*w(x, y, z) = w*0
(2.1)

*where u, v, w represent displacement components in the x, y and z directions, respectively;*
*and u*0*, v*0*, w*0 *are displacement components in the middle surface of the plate. θx* *and θy* are
*rotations about the y and x axes at the mid-plane, respectively. The ﬁrst order derivatives of*
the transverse displacement can be formulated in terms of the in-plane displacement parameters
as separate independent degrees of freedom as given below

*u(x, y, z) = u*0*(x, y) − zφx(x, y) + [g(z) + Γ z]θx(x, y)*
*v(x, y, z) = v*0*(x, y) − zφy(x, y) + [g(z) + Γ z]θy(x, y)*
*w(x, y, z) = w*0*(x, y)*
(2.2)
where
*φx* = *∂w*
*∂x* *φy* =
*∂w*
*∂y* *g(z) = sin*
*πz*
*h* exp
*m cosπz*
*h*
*Γ =* *π*
*hm*

The linear displacement vector given in the above equation can be expressed in terms of the middle surface of the laminated plate as follows

**ε**_{5×1}**= Z*** _{5×13}ε_{13×1}* (2.3)
where

*= n*

**ε***ε*0 1

*ε*02

*ε*06

*κ*11

*κ*12

*κ*16

*ε*04

*ε*05

*κ*24

*κ*25 oT

*ε*0

_{1}=

*∂u*0

*∂x*

*ε*0 2 =

*∂v*0

*∂y*

*ε*0 6 =

*∂u*0

*∂y*+

*∂v*0

*∂x*

*ε*0 4 =

*∂w*0

*∂y*

*− φy*

*ε*0

_{5}=

*∂w*0

*∂x*

*− φx*

*k*0 1

*= Γ*

*∂θx*

*∂x*

*−*

*∂φx*

*∂x*

*k*0 2

*= Γ*

*∂θy*

*∂y*

*−*

*∂φy*

*∂y*

*k*

_{6}0

*= Γ*

*∂θx*

*∂y*+

*∂θy*

*∂y*

*−∂φx*

*∂y*

*−*

*∂φy*

*∂x*

*k*1 1 =

*∂θx*

*∂x*

*k*1 2 =

*∂θy*

*∂x*

*k*

_{6}1 =

*∂θy*

*∂x*+

*∂θx*

*∂y*

*k*2 4

*= θy*

*k*52

*= θx*

**Z =**
*1 0 0 z 0 0 g(z)* 0 0 0 0 0 0
*0 1 0 0 z 0* 0 *g(z) 0* 0 0 0 0
*0 0 1 0 0 z* 0 0 *0 g(z) 0* 0 0
0 0 0 0 0 0 0 0 0 1 *0 g(z)* 0
0 0 0 0 0 0 0 0 0 0 1 0 *g(z)*
and
**ε**_{13×1}**= L**_{13×7}**∆**_{7×1}**∆ =**
n
*u*0 *v*0 *w*0 *θx* *θy* *φx* *φy*
oT

The following assumptions are considered in the derivation of the equations:

*• Small elastic deformations are assumed (i.e. deformations and rotations are small and agree*
to the Hooke’s law).

*• The plies of the composite laminated structure are supposed to be well bonded.*

The linear strain equations derived from the displacements of Eqs. (2.1), which are valid for thin as well as thick plates under consideration, are as follows

*εxx= ε*0* _{xx}+ zε*1

*+ sin*

_{xx}*πz*

*h*exp

*m cosπz*

*h*

*ε*2

_{xx}*εyy= ε*0

*1*

_{yy}+ zε*+ sin*

_{yy}*πz*

*h*exp

*m cosπz*

*h*

*ε*2

_{yy}*εxy*

*= ε*0

*1*

_{xy}+ zε*+ sin*

_{xy}*πz*

*h*exp

*m cosπz*

*h*

*ε*2

_{xy}*εxz*

*= ε*0

*+*

_{xz}*π*

*h*cos

*πz*

*h*

*− m sin*2

*πz*

*h*exp

*m cosπz*

*h*

*ε*3

_{xz}*εyz= ε*0

*+*

_{yz}*π*

*h*cos

*πz*

*h*

*− m sin*2

*πz*

*h*exp

*m cosπz*

*h*

*ε*3

*(2.4) and*

_{yz}*ε*0

*=*

_{xx}*∂u*

*∂x*

*ε*1

*xx*

*= m*

*π*

*h*

*∂θx*

*∂x*

*−*

*∂*2

_{w}*∂x*2

*ε*2

*xx*=

*∂θx*

*∂x*

*ε*0

*=*

_{yy}*∂v*

*∂x*

*ε*1

*yy*

*= m*

*π*

*h*

*∂θy*

*∂x*

*−*

*∂*2

*w*

*∂x*2

*ε*2

*yy*=

*∂θy*

*∂x*

*ε*0

*=*

_{xy}*∂v*

*∂x*+

*∂u*

*∂y*

*ε*1

*xy*

*= m*

*π*

*h*

*∂θy*

*∂x*

*+ m*

*π*

*h*

*∂θx*

*∂y*

*− 2*

*∂*2

*w*

*∂x∂y*

*ε*2

*xy*=

*∂θy*

*∂x*+

*∂θx*

*∂y*

*ε*0

*xz*

*= m*

*π*

*hθx*

*ε*3

*xz*

*= θx*

*ε*0

*yz= m*

*π*

*hθy*

*ε*3

*yz*

*= θy*(2.5)

**3.** **Governing equations of the hygrothermal buckling and post-buckling**
The laminated plate composed of elastic orthotropic plies and the stress–strain relations in the
orthotropic local frame are as follows (Reddy, 2004)

*σ*1
*σ*2
*τ*12
*τ*13
*τ*23
=
*Q*11 *Q*12 0 0 0
*Q*12 *Q*22 0 0 0
0 0 *Q*66 0 0
0 0 0 *Q*55 0
0 0 0 0 *Q*44
*ε*1
*ε*2
*γ*12
*γ*13
*γ*23
(3.1)

*where Qij* are elastic stiﬀness coeﬃcients relative to the plane-stress state that neglects the
transversal stress. These coeﬃcients are given below (Reddy, 2004) in terms of the engineering
constants in the material coordinates

*Q*11= *E1*
*1 − ν*12*ν*21
*Q*22= *E2*
*1 − ν*12*ν*21
*Q*12*= ν*12*Q*11 *Q*33*= G*12
*Q*44*= G*23 *Q*55*= G*13 *ν*21*= ν*12
*E*2
*E*1
(3.2)

In general, the laminates are in the plane stress state due to temperature or moisture changes; therefore, externally applied stresses would develop at the supports. These in-plane stresses can be evaluated using elasto-hygrothermal constitutive equation. When hygrothermal eﬀects are considered, the stress tensor is usually expressed in the contracted notation as follows

*σi= Qij* *εj−*
*T*
Z
*T*0
*αj(τ, M ) dτ −*
*M*
Z
*M*0
*βj(T, m) dm*
!
*i, j = 1, 2, 3* (3.3)

*where the elastic stiﬀness coeﬃcients Qij, the thermal expansion coeﬃcients αj*, and the
*moistu-re coeﬃcients βj* *depend upon the temperature T and moisture concentration M . For moderate*
*temperature ∆T = T − T*0 *and moisture ∆M = M − M*0 changes from the corresponding
*stress--free values T*0 *and M*0, if the elastic properties are considered independent from the
hygrother-mal, the stress-strain relations are simpliﬁed as follows

*σ = Qij(ε*1*− αj∆T − β∆M)(ε1− αj∆T − β∆M)* *i, j = 1, 2, 3* (3.4)
Proper tensor transformations can be employed in transforming equation (3.4) from principal
*material coordinates x*1*, x*2 *and x*3 *to the plate coordinates x, y and z. For a typical k-th ply of*
the laminate, the resulted expression can be written as

*σxx*
*σyy*
*τxy*
*τxz*
*τyz*
*k*
=
*Q*_{11} *Q*_{12} *Q*_{16} 0 0
*Q*_{12} *Q*_{22} *Q*_{26} 0 0
*Q*_{16} *Q*_{26} *Q*_{66} 0 0
0 0 0 *Q*_{55} *Q*_{54}
0 0 0 *Q*_{45} *Q*_{44}
*k*
*εxx− αx∆T − βx∆C*
*εyy− αy∆T − βy∆C*
*εxy− αxy∆T − βxy∆C*

*εxz*
*εyz*
*k*
(3.5)
or in a condensed form
**σ**_{k}**= Q*** _{k}ε_{k}* (3.6)

*where Qij, αi, βi* *(i, j = x, y, xy) denote the transformed material coeﬃcients.*

According to the potential energy theorem, the equilibrium state can be achieved when variation of the total potential energy equates to zero.

*The potential energy theorem can be expressed for the typical i-th ply enclosing a space*
*volume V as follows*

Z

*V*

*(σxxδεxx+ σyyδεyy+ τxyδεxy+ τxzδεxz* *+ τyzδεyz) dVe−*

Z

*A*

*qδw dAe*= 0 (3.7)

When the laminate is subjected to temperature or moisture changes, due to the restriction on freeing the hygrothermal loading, some stresses are developed at the supports. The governing equations on the pre-buckling can be obtained via the following formula

**K∆ = F** (3.8)

**where K is the linear stiﬀness matrix and F represents the load vector associated with the **
tem-perature variation or hygroscopic eﬀects. Equation (3.8) is solved under the speciﬁed boundary
**condition and in-plane loads. In the next step, the geometric stiﬀness matrix K***G* associated

with these in-plane loads is calculated. The critical hygrothermal buckling is calculated through solving the linear eigenvalue problem

**(K + λ**cr**K***G***)∆ = 0** (3.9)

The smallest eigenvalue corresponds to the amplitude of the critical buckling load. In the
**post--buckling step, the nonlinear stiﬀness matrix K***nl* is incorporated as

**(K + K***nl+ λcr***K***G***)∆ = 0** (3.10)

The geometric stiﬀness matrix can be expressed as

**K***G= σxp***K***G1+ σpy***K***G2* (3.11)

*where σp*

*x, σpy* *denote externally applied stresses acting in the x and y directions. Subsequently,*
the critical buckling stresses can be calculated by the following formulas

*σp _{xc}r = λcrσp_{x}*

*σ*

_{y c}p*r = λcrσ*(3.12)

_{y}p**4.** **Numerical results and discussion**

In this Section, numerical examples are presented for buckling and post buckling of the laminated composite plates under mechanical and hygrothermal loads. The accuracy of the proposed TSDM model considering the transverse shear stresses is examined. A variety of problems are solved using the ﬁnite element formulation and the results are compared with 3D elasticity solution. It is important to note that the proposed displacement model can be applied to any lay-up of the laminated plates. The diﬀerent mechanical properties examined in the numerical examples are given in Table 1.

**Table 1. Material properties used in the numerical examples**

Mater- Elastic constants

ial No. (Reddy and Liu, 1985; Dafedar and Desai, 2002)
1 *E*1*/E*2 *= 25, G*12*= G*13*= 0.5E*2*, G*23*= 0.2E*2*, ν*12*= 0.25*

2 *E*1*/E*2 *= 3 to 40, E*3*= E*2*, G*12*/E*2 *= G*13*/E*2*= 0.60, G*23*/E*2 *= 0.50,*
*ν12= ν*23*= ν*13*= 0.25*

3 *E1/E2* *= 40, E*3 *= E*2*, G*12/E2 *= G*13/E2 *= 0.50, G*23/E2*= 0.20,*
*ν*12*= ν*23*= ν*13*= 0.25*

4 *E*1*/E*2 *= 15, E*3 *= E*2*, G*12*/E*2 *= G*13*/E*2 *= 0.50, G*23*/E*2*= 0.3356,*
*ν*12*= ν*23*= ν*13*= 0.3, a*1*/a*0*= 0.015, a*2*/a*0 *= a*3*/a*0 *= 1.00*

5 Elastic moduli of graphite/epoxy ply at diﬀerent moisture
*concentrations C [%],*

*E1* *= 130 GPa, G*13*= G*12*= 6.0 GPa, G*23*= 0.5G*12,
*ν*12*= ν*23*= ν*13*= 0.3, β*1 *= 0 and β*2 *= β*3 *= 0.44 and*

*C [%]* 0.00 0.25 0.50 0.75 1.00 1.25 1.50
*E*2 [GPa] 9.50 9.25 9.00 8.75 8.50 8.50 8.50

In order to simplify comparison, the critical buckling stresses have been transformed into dimensionless coeﬃcients as follows

*λcr* =
*σcrb*2

**4.1.** **Examples for validating the TSDM model**

Three cases are examined to conﬁrm TSDM formulation using ﬁnite element programming.
**Case A**

A symmetric four-layered (0/90/90/0) cross-ply laminated plate is considered under uniaxial
compression loading. The critical buckling coeﬃcients for various values of length-to-thickness
*ratios a/h are presented in Table 2. As it is demonstrated in Table 2, the HSDT overestimates*
the critical buckling loads in comparison with the results from the present formulation and those
*given by Pagano et al. (1994).*

**Table 2. Eﬀect of length to thickness ratio on the critical buckling load**

*a/h* Present 3D HSDT

(Pagano and Reddy, 1994) (Reddy and Liu, 1985)

5 1.922 1.575 1.997
10 13.367 13.453 13.384
20 20.689 21.707 21.886
50 23.354 23.356 23.747
100 24.034 24.255 24.953
**Case B**

The eﬀect of elastic moduli ratios on the buckling loads of a square plate under uniaxial loading is examined, and the results are presented in Table 3. According to the results obtained via the TSDM formulation are in excellent agreement with other references.

**Table 3. Eﬀect of elastic moduli ratios on critical buckling loads**

*E*1*/E*2 Present _{(Pagano and Reddy, 1994)}3D _{(Reddy and Liu, 1985)}HSDT

3 5.396 5.399 5.114
10 9.952 9.967 13.384
20 15.327 15.352 15.297
30 19.703 19.758 19.968
40 23.564 23.451 23.344
**Case C**

Table 4 presents the comparison between the critical buckling coeﬃcients obtained through
the present model and the reference values for the square laminated plate under uniaxial
*com-pression loading. The analysis is carried out for two values of ﬁber orientation angles θ = 30◦*
*and θ = 45◦*

for both of the two-ply and six-ply antisymmetric angle-ply laminates. The results are validated by comparing them with the HSDT model proposed by Reddy and Liu (1985).

**4.2.** **Effect of the length-to-thickness ratio on the critical buckling load**

A symmetric four-layered (0/90)s cross-ply laminated plate is considered under both uniaxial and biaxial compression loadings. The eﬀect of the side-to-thickness ratio for the simply suppor-ted rectangular plate is examined using material No. 1, and the results are plotsuppor-ted in Fig.1. It is

**Table 4. Critical buckling coeﬃcients for angle-ply laminates**
*θ = 30◦*

*θ = 45◦*

*a/h* 2 ply 6 ply *a/h* 2 ply 6 ply

Present [10] Present [10] Present [10] Present [10] 5 10.694 11.543 13.404 13.536 5 10.084 10.782 12.169 12.172 10 16.108 17.123 29.046 33.624 10 16.734 18.051 30.648 32.504 20 18.234 18.764 41.023 46.231 20 19.234 19.764 48. 230 52.132 50 19.748 19.863 49.963 51.643 50 20.746 20.863 58.963 59.643 100 20.308 30.603 53.079 54.896 100 21.267 21.664 59.431 61.021 [10] – Muc and Chwał (2016)

observed that the critical buckling loads are higher in the uniaxial loading case. Additionally, the
buckling load coeﬃcients increase considerably as the thickness ratio decreases. The variations
*of both curves for two loading conditions are very slow above the a/h = 40 ratio (are only a*
*little above a/h = 40).*

Fig. 1. Eﬀect of the length-to-thickness ratio on the critical buckling load for cross-ply laminates

**4.3.** **Effect of ply orientation on the critical buckling load**

The buckling load coeﬃcient for a square and antisymmetric angle-ply laminated plate is tested under uniaxial compressive loading; the eﬀect of ply orientation for various numbers of layers of the angle-ply laminate is plotted in Fig. 2. All the edges are supposed to be simply supported, and material 5 of Table 1 is used in all cases. It is observed that in all cases, the

critical buckling load increases at ﬁrst but decreases then. By varying the ﬁber orientation angles
from 0*◦*

to 90*◦*

, it is observed that the maximum critical buckling load occurs at 45*◦*
.

**4.4.** **Effect of the elastic moduli ratio on the critical buckling load**

The variations of critical buckling coeﬃcients of antisymmetric cross-ply laminated plates
under uniaxial and biaxial loadings are demonstrated in Figs. 3, respectively. The results are
*presented for a/h = 10. It is observed that as the elastic moduli ratio rises, the critical buckling*
load also increases in both uniaxial and biaxial loadings; however, in biaxial cases, the buckling
loads are approximately half of the corresponding uniaxial values at all analyzed ratios.

*Fig. 3. Variation of the buckling load for square antisymmetric cross-ply laminate when a/h = 10;*
(a) uniaxial loading, (b) biaxial loading

**4.5.** **Effect of thermal loads on the buckling of laminates**

Buckling under thermal loads for a laminated plate consisting of 10 plies of material 4 is
examined using TSDM model and compared with 3D elasticity solutions. The thermal buckling
*coeﬃcients of λT* *= α*0*Tcr* are provided in Table 5. The obtained results are in excellent agreement
with the 3D elasticity results proposed by Noor and Burton (1992), for both the thin and thick
laminated plates. In this case, the critical buckling loads correspond to the buckling modes
*of m, n = 1, 2, because the laminates under high temperature variations are mainly subjected*
to the biaxial loading condition. The results conﬁrm that the buckling in the thick laminated
plates occur at higher temperatures compared to the thin ones. In Fig. 4, the thermo-buckling
*curve is plotted for a simply supported square and [±45◦*

] antisymmetric angle-ply laminate.
The obtained results by the present model are very close to the analytical solutions proposed
*by Singha et al. (2001).*

**Table 5. Thermal buckling coeﬃcient λ**T*= α*0*Tcr* for a square angle-ply laminated plate

*a/h* Present 3D solution
(Noor and Burton, 1992)
100.0000 *0.7463 · 10−*3
*0.7458 · 10−*3
20.0000 *0.1739 · 10−*_{3}
*0.1721 · 10−*_{3}
10.0000 *0.5782 · 10−*3
*0.5820 · 10−*3
6.6667 0.1029 0.1034
5.0000 0.1436 0.1515
4.0000 0.1777 0.1886
3.3333 0.2057 0.2063

*Fig. 4. Thermo-buckling path plotted for a simply supported square [±45◦*_{] antisymmetric}
angle-ply laminate

**4.6.** **Effect of change in moisture concentration on the buckling load**

*The eﬀects of changes in moisture concentrations on the uniaxial buckling load coeﬃcients λU*
*of a cross-ply [(0/90)s*] laminate using material 5 is presented in Table 6. The buckling loads
are evaluated by reducing the material properties and increasing the moisture concentration.
*The parameter (E*2)*c=0%* *is used to calculate the buckling load coeﬃcient λU* using the TSDM
model. In Fig. 6, the variation of the buckling load coeﬃcient with respect to the moisture
*concentration is shown for diﬀerent b/h ratios. As it is seen from this ﬁgure, in thin plates, the*
buckling coeﬃcient decreases faster compared to the thick ones. However, the slope is almost
linear for both thin and thick laminates, and the thin plates may buckle due to a little change
in the moisture concentration, even in the absence of external loads.

**Table 6. Eﬀect of moisture concentration on the critical buckling load coeﬃcient of a symmetric**
cross-ply laminated plate for various values of the thickness-to-length ratio

*a/h* *C [%]* Present Dafedar and Desai (2002)

5 0.0 6.9932 7.1383 0.5 6.8911 7.0365 1.0 6.7963 6.9420 1.5 6.7320 6.8776 10 0.0 11.3466 11.4275 0.5 11.0183 11.0990 1.0 10.7205 10.8009 1.5 10.4631 10.5435 20 0.0 13.6835 13.7106 0.5 12.5247 12.5517 1.0 11.4879 11.5147 1.5 10.4582 10.4851 40 0.0 14.4529 14.4602 0.5 10.0180 10.0254 1.0 6.0708 6.0781 1.5 1.9523 1.9596

**5.** **Conclusions**

A new ﬁnite element formulation is developed using MHSDT for investigating the eﬀects of elasto-hygrothermal loads in the buckling of composite laminated plates. The transverse stresses through thickness of a plate and the continuity of displacements are entirely satisﬁed in the proposed formulation. From the extensive numerical investigation, the results obtained using Trigonometric Shear Displacement Model (TSDM) is in excellent agreement with the three--dimensional elasticity solutions as well as other equivalent higher-order theories. The variations of the critical buckling load are presented for diﬀerent lamination lay-ups, elastic constants and length-to-thickness plate ratios. The eﬀect of thermally-induced loading and moisture concen-tration on the buckling and post-buckling of the laminated plates are investigated using TSDM formulation. The following conclusions are obtained:

*• In the hygrothermal buckling analysis of composite plates, it is mandatory to exploit*
reﬁned higher-order theories dealing with the transverse normal deformation.

*• Increasing the moisture concentrations and temperatures would result in a reduction in the*
buckling and post-buckling strength. The results also conﬁrm that the post-buckling
cha-racteristics are signiﬁcantly aﬀected by a rise in the temperature, moisture concentration,
transverse shear deformation, plate geometry, total number of plies and ﬁber orientation.
*• Increasing the length-to-thickness ratio, the number of layers and the orthotropic ratio*
*(E*1*/E*2) would lead to an increase in the buckling strength due to in-plane compressive
loading.

*• The critical buckling load is higher in the case of uniaxial loading compared to the biaxial*
one.

**References**

*1. Agarwal B.D., Broutman L.J., Chandrashekhara K., 2006, Analysis and Performance of*
*Fiber Composites, 3rd ed., Wiley, New York*

2. Ahmadi S.A., Pourshahsavari H., 2016, Three-dimensional thermal buckling analysis of
*functio-nally graded cylindrical panels using diﬀerential quadrature method (DQM), Journal of Theoretical*
*and Applied Mechanics, 54, 1, 135-147*

3. Brischetto S., 2013, Hygrothermoelastic analysis of multilayered composite and sandwich shells,
*Journal of Sandwich Structures and Materials, 15, 2, 168-202*

4. Dafedar J.B., Desai Y.M., 2002, Thermomechanical buckling of laminated composite plates
* using mixed, higher-order analytical formulation, Journal of Applied Mechanics, 69, 6, 790-799*
5. Girish J., Ramachandra L.S., 2005, Thermomechanical post-buckling analysis of symmetric

* and antisymmetric composite plates with imperfections, Composite Structures, 67, 4, 453-460*
6. Kazemi M., Verchery G., 2016, Design of composite laminated plates for maximum buckling

**load with stiﬀness and elastic modulus constraints, Composite Structures, 148, 27-38**

7. Kharazi M., Ovesy H.R., Mooneghi M.A., 2014, Buckling analysis of delaminated composite
**plates using a novel layerwise theory, Thin-Walled Structures, 74, 246-254**

8. Mantari J.L., Oktem A.S., Soares C.G., 2012, A new higher order shear deformation theory
* for sandwich and composite laminated plates, Composites Part B: Engineering, 43, 3, 1489-1499*
9. Mechab B., Mechab I., Benaissa S., 2012, Analysis of thick orthotropic laminated

compo-site plates based on higher order shear deformation theory by the new function under
**thermo-mechanical loading, Composites Part B: Engineering, 43, 3, 1453-1458**

10. Muc A., Chwał M., 2016, Analytical discrete stacking sequence optimization of rectangular
*composite plates subjected to buckling and FPF constraints, Journal of Theoretical and Applied*
*Mechanics, 54, 2, 423-436*

11. Natarajan S., Deogekar P.S., Manickam G., Belouettar S., 2014, Hygrothermal eﬀects
*on the free vibration and buckling of laminated composites with cutouts, Composite Structures,*

**108, 848-855**

12. Noor A.K., Burton W.S., 1992, Three-dimensional solutions for thermal buckling of
**multilay-ered anisotropic plates, Journal of Engineering Mechanics, 118, 4, 683-701**

*13. Pagano N.J., Reddy J.N., 1994, Mechanics of Composite Materials: Selected Works of Nicholas*
*J. Pagano, 34, Springer Science & Business Media*

14. Pandey R., Upadhyay A.K., Shukla K.K., 2009, Hygrothermoelastic postbuckling response of
**laminated composite plates, Journal of Aerospace Engineering, 23, 1, 1-13**

15. Peković O., Stupar S., Simonović A., Svorcan J., Trivković S.A., 2015, Free vibration
and buckling analysis of higher order laminated composite plates using the isogeometric approach,
*Journal of Theoretical and Applied Mechanics, 53, 2, 453-466*

16. Reddy J.N., Liu C.F., 1985, A higher-order shear deformation theory of laminated elastic shells,
*International Journal of Engineering Science, 23, 3, 319-330*

*17. Reddy J.N., 2004, Mechanics of Laminated Composite Plates and Shells, 2nd ed., CRC Press*
18. Singha M.K., Ramachandra L.S., Bandyopadhyay J.N., 2001, Thermal post-buckling

**ana-lysis of laminated composite plates, Composite Structures, 54, 4, 453-458**

19. Sreehari V.M., Maiti D.K., 2015, Buckling and post buckling analysis of laminated
compo-site plates in hygrothermal environment using an Inverse Hyperbolic Shear Deformation Theory,
*Composite Structures, 129, 250-255*

*20. Tauchert T., Huang N., 2012, Laminated Plates, Composite Structures 4: Volume 1 Analysis*
*and Design Studies, 424*

*21. Turvey G.J., Marshall I.H., Eds., 2012, Buckling and Postbuckling of Composite Plates, *
Sprin-ger Science & Business Media, Netherlands